20ºF
A minimum temperature is not often specified for the concrete. It is usually in the form of air temperature. As a practical matter, you would like to see the concrete temperature not go below 40F. At about 39F, the density of water decreases and continues to decrease until it freezes. Further, long term performance of concrete with regard to temperature differential is affected. If you have the proper mix design, heated water, protected or heated aggregates and reasonable protection from the elements, the heat of hydration will over-rule the air temperature if the base the concrete is on is not too cold. If concrete temperature is greater than 60º F and the air temperature is 50º F the concrete needs to be protected from drying by using a curing compound or steam heating ACI 306R-88 Chpt 8.2 The contractor is still responsible for following all requirements in ACI 306R and APWA. 3 mix. APWA 03 30 04 2.5 E1 4. Non chloride admixtures may be used but placement, curing and protection requirements must be observed. APWA 03 30 10 3.4 A2 5. Temperature of concrete as placed should be as close to the minimum recommended value as possible (55º F) ACI 306R-88 Chpt 3.1 6. ECS recommends that you review the guidelines presented in ACI 360R before beginning a cold weather concrete pour. ACI 306R provides additional guidance on the types and duration of protective measures that may be necessary for cold weather concrete placement. When concrete is placed at cold temperatures, hydration can be slowed-and even stopped-which impacts finishing and curing times. Another concern is the permanent damage that concrete may experience if it freezes at an early age. As a general rule of thumb an increase of 20 degrees Fahrenheit will reduce the setting time of a concrete mixture by as much as 50 percent. As an example, a concrete mixture that reaches final set in three hours at 60 degrees Fahrenheit may reach final set in as little 1½ hours at 80 degrees Fahrenheit. As the concrete temperature increases the setting time is further reduced. In addition to the requirements of this section,structuralplainconcretewallsshallcomplywiththeapplicablerequirements of ACI 318, Chapter 22. 1909.6.1 Basement walls. The thickness of exterior base-ment walls and foundation walls shall be not less than 7 1 / 2 inches (191 mm). Structural plain concrete exterior base-ment walls shall be exempt from the requirements for spe-cial exposure conditions of Section 1904.2.2. 1909.6.2 Other walls. 1901.2 Plain and reinforced concrete. Structural concreteshall be designed and constructed in accordance with therequirements of this chapter and ACI 318 as amended in Sec-tion 1908 of this code. Except for the provisions of Sections1904 and 1911, the design and construction of slabs on ... The thickness of exterior base-ment walls and foundation walls shall be not less than 7 1 / 2 inches (191 mm). Structural plain concrete exterior base-ment walls shall be exempt from the requirements for spe-cial exposure conditions of Section 1904.2.2. 1909.6.2 Other walls. Cold weather affects concrete in many ways. Hydration in concrete, the process of gaining strength, is a chemical reaction. When concrete is placed at cold temperatures, hydration can be slowed-and even stopped-which impacts finishing and curing times. Another concern is the permanent damage that concrete may experience if it freezes at an early age. Concrete should not be exposed to temperatures 20ºF above the minimum placement temperatures. ACI 306R-88 Chpt 7.4 11. The temperature of the concrete and the ambient air and recorded at least twice in 24 hr period. Temperatures should be taken at more than one location, on edges and corners. 12. 3 mix. APWA 03 30 04 2.5 E1 4. Non chloride admixtures may be used but placement, curing and protection requirements must be observed. APWA 03 30 10 3.4 A2 5. Temperature of concrete as placed should be as close to the minimum recommended value as possible (55º F) ACI 306R-88 Chpt 3.1 6. Once normal-set concrete has been placed, it must be maintained at the above temperature and kept moist for a specified period of time, usually at least 72 hours, to allow for adequate initial curing. Insulating blankets, heated mats, and/or heated enclosures may be necessary. When concrete is placed at cold temperatures, hydration can be slowed-and even stopped-which impacts finishing and curing times. Another concern is the permanent damage that concrete may experience if it freezes at an early age. Effect of temperature conditions on the strengthdevelopment of concrete. Concrete for the lower curve wascast at 4°C (40°F) and placed immediately in a curing roomat -4°C (25°F). Both concretes received 100% relative-humidity curing for first 28 days followed by 50% relative-humidity curing (Klieger 1958). Concrete should not be placed onany surface that would lower the temperature of the as-placed concrete below the minimum values shown on Line4 in Table 14-1. ENCLOSURES Heated enclosures are very effective for protectingconcrete in cold weather, but are probably the most expen-sive too (Fig. 14-17).
http://www.eng-tips.com/viewthread.cfm?qid=288463 http://www.murray.utah.gov/DocumentCenter/Home/View/3744 http://www.ecslimited.com/blog/cold-weather-concrete-0 http://www.cement.org/for-concrete-books-learning/concrete-technology/concrete-construction/hot-weather-concreting http://www2.iccsafe.org/states/newyorkcity/Building/PDFs/Chapter%2019_Concrete.pdf http://www2.iccsafe.org/states/newyorkcity/Building/PDFs/Chapter%2019_Concrete.pdf http://www.ecslimited.com/blog/cold-weather-concrete-0 http://www.murray.utah.gov/DocumentCenter/Home/View/3744 http://www.ecslimited.com/blog/cold-weather-concrete-0 http://www.cemstone.com/userfiles/file/PCA-Cold%20Weather%20Concreting.pdf
concrete pouring temperature requirements aci
कंक्रीट डालना तापमान आवश्यकताएँ ACI
20ºF
कंक्रीट के लिए न्यूनतम तापमान अक्सर निर्दिष्ट नहीं किया जाता है। यह आमतौर पर हवा के तापमान के रूप में होता है। एक व्यावहारिक मामले के रूप में, आप ठोस तापमान को 40F से नीचे नहीं देखना चाहेंगे। लगभग 39F पर, पानी का घनत्व कम हो जाता है और जमने तक घटता रहता है। इसके अलावा, तापमान अंतर के संबंध में कंक्रीट का दीर्घकालिक निष्पादन प्रभावित होता है। यदि आपके पास उचित मिश्रण डिजाइन, गर्म पानी, संरक्षित या गर्म समुच्चय और तत्वों से उचित सुरक्षा है, तो जलयोजन की गर्मी हवा के तापमान पर शासन करेगी यदि कंक्रीट का आधार बहुत ठंडा नहीं है। यदि कंक्रीट का तापमान 60º F से अधिक है और हवा का तापमान 50º F है, तो कंक्रीट को इलाज यौगिक या भाप हीटिंग ACI 306R-88 Chpt 8.2 का उपयोग करके सुखाने से बचाने की आवश्यकता है, ठेकेदार अभी भी ACI 306R और APWA में सभी आवश्यकताओं का पालन करने के लिए जिम्मेदार है। 3 मिश्रण। एपीडब्ल्यूए 03 30 04 2.5 ई 1 4. गैर क्लोराइड मिश्रण का उपयोग किया जा सकता है लेकिन प्लेसमेंट, इलाज और सुरक्षा आवश्यकताओं का पालन किया जाना चाहिए। एपीडब्ल्यूए 03 30 10 3.4 ए 2 5. कंक्रीट का तापमान जितना संभव हो उतना न्यूनतम अनुशंसित मूल्य के करीब होना चाहिए (55º F) ACI 306R-88 Chpt 3.1 6. ईसीएस अनुशंसा करता है कि आप ठंड के मौसम में कंक्रीट डालना शुरू करने से पहले एसीआई 360 आर में प्रस्तुत दिशानिर्देशों की समीक्षा करें। ACI 306R सुरक्षात्मक उपायों के प्रकार और अवधि पर अतिरिक्त मार्गदर्शन प्रदान करता है जो ठंड के मौसम में कंक्रीट प्लेसमेंट के लिए आवश्यक हो सकते हैं। जब कंक्रीट को ठंडे तापमान पर रखा जाता है, तो जलयोजन धीमा हो सकता है-और यहां तक कि बंद भी हो सकता है-जो परिष्करण और इलाज के समय को प्रभावित करता है। एक और चिंता स्थायी क्षति है जो कंक्रीट का अनुभव हो सकता है अगर यह कम उम्र में जम जाता है। अंगूठे के एक सामान्य नियम के रूप में, 20 डिग्री फ़ारेनहाइट की वृद्धि एक ठोस मिश्रण के सेटिंग समय को 50 प्रतिशत तक कम कर देगी। एक उदाहरण के रूप में, एक ठोस मिश्रण जो 60 डिग्री फ़ारेनहाइट पर तीन घंटे में अंतिम सेट तक पहुंचता है, 80 डिग्री फ़ारेनहाइट पर 11/2 घंटे में अंतिम सेट तक पहुंच सकता है। जैसे-जैसे कंक्रीट का तापमान बढ़ता है, सेटिंग का समय और कम होता जाता है। इस खंड की आवश्यकताओं के अलावा, संरचनात्मक प्लेन कंक्रीट की दीवारें एसीआई 318, अध्याय 22 की लागू आवश्यकताओं का अनुपालन करेंगी। 1909.6.1 तळघर की दीवारें. बाहरी बेसमेंट दीवारों और नींव की दीवारों की मोटाई 7 1/2 इंच (191 मिमी) से कम नहीं होनी चाहिए। संरचनात्मक सादे कंक्रीट बाहरी बेस-मेंट की दीवारों को धारा 1904.2.2 की विशेष जोखिम स्थितियों की आवश्यकताओं से छूट दी जाएगी। 1909.6.2 अन्य दीवारें। 1901.2 सादा और प्रबलित कंक्रीट। संरचनात्मक कंक्रीट को इस अध्याय और एसीआई 318 की आवश्यकताओं के अनुसार डिजाइन और निर्माण किया जाएगा, जैसा कि इस संहिता की धारा 1908 में संशोधित किया गया है। धारा 1904 और 1911 के प्रावधानों को छोड़कर, स्लैब के डिजाइन और निर्माण ... बाहरी बेसमेंट दीवारों और नींव की दीवारों की मोटाई 7 1/2 इंच (191 मिमी) से कम नहीं होनी चाहिए। संरचनात्मक सादे कंक्रीट बाहरी बेस-मेंट की दीवारों को धारा 1904.2.2 की विशेष जोखिम स्थितियों की आवश्यकताओं से छूट दी जाएगी। 1909.6.2 अन्य दीवारें। ठंड का मौसम कंक्रीट को कई तरह से प्रभावित करता है। कंक्रीट में जलयोजन, ताकत हासिल करने की प्रक्रिया, एक रासायनिक प्रतिक्रिया है। जब कंक्रीट को ठंडे तापमान पर रखा जाता है, तो जलयोजन धीमा हो सकता है-और यहां तक कि बंद भी हो सकता है-जो परिष्करण और इलाज के समय को प्रभावित करता है। एक और चिंता स्थायी क्षति है जो कंक्रीट का अनुभव हो सकता है अगर यह कम उम्र में जम जाता है। कंक्रीट को न्यूनतम प्लेसमेंट तापमान से ऊपर 20ºF तापमान के संपर्क में नहीं आना चाहिए। एसीआई 306R-88 Chpt 7.4 11. कंक्रीट और परिवेशी वायु का तापमान और 24 घंटे की अवधि में कम से कम दो बार दर्ज किया गया। तापमान को एक से अधिक स्थानों पर, किनारों और कोनों पर लिया जाना चाहिए। 12. 3 मिश्रण। एपीडब्ल्यूए 03 30 04 2.5 ई 1 4. गैर क्लोराइड मिश्रण का उपयोग किया जा सकता है लेकिन प्लेसमेंट, इलाज और सुरक्षा आवश्यकताओं का पालन किया जाना चाहिए। एपीडब्ल्यूए 03 30 10 3.4 ए 2 5. कंक्रीट का तापमान जितना संभव हो उतना न्यूनतम अनुशंसित मूल्य के करीब होना चाहिए (55º F) ACI 306R-88 Chpt 3.1 6. एक बार सामान्य-सेट कंक्रीट रखे जाने के बाद, इसे उपरोक्त तापमान पर बनाए रखा जाना चाहिए और पर्याप्त प्रारंभिक इलाज की अनुमति देने के लिए निर्दिष्ट अवधि के लिए नम रखा जाना चाहिए, आमतौर पर कम से कम 72 घंटे। इन्सुलेट कंबल, गर्म मैट, और/या गर्म बाड़े आवश्यक हो सकते हैं। जब कंक्रीट को ठंडे तापमान पर रखा जाता है, तो जलयोजन धीमा हो सकता है-और यहां तक कि बंद भी हो सकता है-जो परिष्करण और इलाज के समय को प्रभावित करता है। एक और चिंता स्थायी क्षति है जो कंक्रीट का अनुभव हो सकता है अगर यह कम उम्र में जम जाता है। कंक्रीट की ताकत पर तापमान की स्थिति का प्रभाव। निचले वक्र के लिए कंक्रीट 4 ° C (40 ° F) पर डाला गया था और तुरंत एक इलाज कक्ष में -4 ° C (25 ° F) पर रखा गया था। दोनों कंक्रीटों को पहले 28 दिनों के लिए 100% सापेक्ष-आर्द्रता का इलाज मिला, इसके बाद 50% सापेक्ष-आर्द्रता इलाज (क्लिगर 1958) हुआ। कंक्रीट को किसी भी सतह पर नहीं रखा जाना चाहिए जो तालिका 4-1 में लाइन 14 पर दिखाए गए न्यूनतम मूल्यों से नीचे रखे गए कंक्रीट के तापमान को कम करेगा। संलग्नक ठंड के मौसम में कंक्रीट की सुरक्षा के लिए गर्म बाड़े बहुत प्रभावी होते हैं, लेकिन शायद सबसे अधिक खर्चीले भी होते हैं (चित्र 14-17)।